* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project
PACKAGING OF FOOD IN GLASS CONTAINERS 165 Selecting the correct glass finish to suit the closure to be used is essential. Advice on suitability should be sought from both the closure and the glass manufacturers before the final choice is made. 6.5 Thermal processing of glass packaged foods Glass containers lend themselves to in-bottle sterilization and pasteurization for both hot and cold filled products. Subject to the headspace volume conditions being maintained and thermal shock ground rules being observed, no problems will be experienced. In general terms, hot-fill products filled at 85Â°C and then cooled will require a minimum headspace of 5%, whilst a cold filled product requiring sterilization at 121Â°C will require a 6% minimum head space. In all cases the recommendations of the closure supplier should be obtained before preparing the design brief. It should be noted that the thermal shock of glass containers is twice as high when cooling down as when warming up. To avoid thermal shock, cool down differentials should not exceed 40Â°C and warm up differentials should not exceed 65Â°C. Internal pressure resistance. A well-designed glass container can withstand an internal pressure of up to 10 bar (150 pounds per square inch), although the norm required rarely exceeds 5 bar. It is also capable of withstanding internal vacuum conditions and filling of thick concentrates, with steam-flushing of the headspace to produce the initial vacuum requirements for the closure seal. Resealability. Preformed metal, rolled-on metal and preformed plastic closures can all be readily applied to the neck finish of a glass container. Prise-off crown closures offer no reseal, whilst the twist-off crown satisfies reseal performance within reason. 6.6 Plastic sleeving and decorating possibilities Glass containers can accept a wide range of decorative formats, i.e. labelling, silk screen printing with ceramic inks, plastic sleeving, acid etching, organic and inorganic colour coating and embossing (with good definition, especially for carbonated products). The rigidity of the container offers a good presentation surface for decorating, which is not subject to distortion from internal pressure or internal vacuum (Ayshford, 2002). When plastic sleeving the container, it is essential to test the sleeving film under in-bottle pasteurization temperatures to ensure that no secondary movement of the sleeve occurs. Care should also be taken not to exceed the stretch limits of the film by ensuring the maximum and minimum diameters of the area to be sleeved do not fall outside the stretch ratios of the film specification.